**Study of the spin correlation and the percolation threshold in the B-site spinel.**

## M. Houssa

^{1}

## , M. Hamedoun

^{*1}

## , N. Benzakour

^{1}

## and A. Hourmatallah

^{2}

## .

*1** Laboratoire de physique du solide. Université Sidi Mohammed Ben Abdellah,Faculté des sciences Dhar*
*Mahraz. B.P. 1796, Fés Atlas- Fés Maroc.*

*2** Groupe de physique du solide, Ecole Normale Superieure, Fés-Maroc.*

High-temperature series expansion of the correlation function on the B- spinel lattice are computed up to order 6 in
*T*

*k*_{B}

= 1

β for Heisenberg model including both the nearest and next-nearest-neighbor interactions J*1* and J*2* respectively.

The behavior with the temperature and the site dilution is presented. The approach is applied to the experimental results of the B-spinel ZnCr2xAl2-2xS4.

The critical temperature and the critical exponents for the susceptibility and the correlation length are deduced by applying the Padé approximant methods. The following estimates are obtained for the familiar critical exponents:

γ* = 1.382*±0.012 and ν* = 0.691*±0.011. These values are not sensitive to the dilution ratio x.

The bond percolation threshold x*p* is determined by studying the disorder variation of the correlation length ξ. The
x_{p} is considered as the concentration at which ξ vanishes. The obtained values are x_{p}=0.27 when only J* _{1}* is
considered and 0.23 when both J

*and J*

_{1}*are considered.*

_{2}**I. INTRODUCTION**

In the last several years, the theoretical and
experimental studies of randomly diluted magnetic
systems have been intensively investigated^{1-6}. In these
systems, non-magnetic ones randomly replace some
magnetic atoms on the lattice and a bond connecting
each pair of occupied atom first neighbor is modified.

In this context, the diluted magnetic systems are associated with a percolation problem when the temperature goes to zero.

In this work, it is intended to extend the development
of the high-temperature series expansion (H.T.S.E) of
the spin correlation functions to the order 6 in β with
nearest-neighbor (n-n) and next-nearest-neighbor (n-n-
n) interactions J* _{1}* and J

*respectively, for the diluted B-spinel lattice ZnCr*

_{2}_{2x}Al

_{2-2x}S

_{4}.

To deduce the spin correlation functions

*)*
*S*
*(*
*S*

*S*
*.*
*S*_{i}_{j}

*ij*= +1

γ

between spins at site i and j we have used the
diagrammatic representation, performed by Stanley
and Kaplan (SK)^{7,8}. Their method is general and can
applied to any lattice. This semi-classical treatment is
a simplification of the more complex procedure of
Rushbrook and Wood^{9} used for the calculation of the
susceptibility in the quantum-mechanical case. In
order to obtain more information about the magnetic
properties in the B-spinel system, we have calculated
the spin correlation functions between first, second
and third n-n, spins γ1* ,*γ* _{2}*and γ

_{3}respectively. We have applied the Padé approximants (P.A) method to the H.T.S.E of the spin correlation function, the magnetic susceptibility χ

*(*

*q*

*)*and the correlation length

*)*
*T*

ξ*(* . The critical temperature T* _{N}*, the critical
exponents γ for the magnetic susceptibility and ν for
the correlation length are deduced. In this whole range
of concentration 0

*.*85≤

*x*≤1, the exponents γ and ν are

found to be equal to 1.382±0.12 and 0.691±0.011 respectively.

It is known that the measurement of the neutron
scattering is a powerful tool for the investigation of
spin correlation^{10,11}. The magnetic ordering of the
diluted system ZnCr_{2x}Al_{2-2x}S_{4} was determined by
neutron diffraction and reported in previous papers^{5,12}.
The main feature of this investigation can be briefly
summarized. In the high concentration *(*0*.*85≤*x*≤1*)* a
long-range magnetic order builds up below the Neel
temperature *T**N*. Below *x*≤0*.*80 no range magnetic
ordering was detected reflecting the spin glass (S.G)
state. No anomaly or saturation was observed at the
freezing temperature T* _{f}* below that the correlation
length ξ still increases.

The inverse correlation length ξ

1 decreases linearly
with temperature leading to a finite value at T=0 in the
S.G state. The nature of the short-range order (S.R.O),
which appears in the concentrated sample above T* _{N}*
and in the S.G samples is of the same type. The S.R.O
is fairly well developed at relatively high-temperature,

*T=100K*

^{5}. The broad diffuse peak of the S.R.O becomes broader and weaker as the temperature is raised corresponding to the thermal disruption of the magnetic correlation. The variation of

*S*

*(*

**q**

*)*, obtained by the H.T.S.E technique with the disorder (variation with temperature T and magnetic site dilution x) is in good accordance with experimental neutron diffraction intensity obtained in the ZnCr

_{2x}Al

_{2-2x}S

_{4}. For a given concentration the location of the broad diffuse peak is insensitive to the temperature

^{5,12,13}. In order to respect this result, the thermal variation of the set of J

*and J*

_{1}*is obtained. Their absolute value decreases with the temperature.*

_{2}The study of the thermal variation of ξ obtained by
the H.T.S.E combined with the experimental
observations in the ZnCr_{2x}Al_{2-2x}S_{4} system permits to

2 143 1999 The Moroccan Statistical Physical Society

derive the variation of ξ with x at T=0. This in turn
also gives us the bond percolation threshold x_{p}. The x_{p}
is considered as the concentration at which ξ
vanishes. The obtained values are x_{p}=0.27 when only
*J** _{1}* is considered and 0.23 when both J

*and J*

_{1}*are considered. These values are in accordance with those obtained by the Monte Carlo method and magnetic experimental results*

_{2}^{14,15}.

**II. THEORY AND RESULTS**

Starting with the zero-field Heisenberg Hamiltonian:

−

=

*j*
*,*
*i*

*j*

*J**ij*

*H* 2 **S**_{i}**.S** (1)

Where the summation run over all pairs of n-n and n-
n-n interactions J* _{1}* and J

*respectively. The expansion of the spin correlation function in powers of β is obtained as follow*

_{2}^{7}.

− =

− = −

=

0

1 αβ

β β

*!*
*)*
*(*
*Tre*

*e*
*Tr*

*H*
*H*
**j**
**i**
**j**
**i**

**.S**
**.S** **S**

**S** (2)

With:

0 1

0 =

−

= − =

−

=ν αµ ν β

α _{m}^{m}

*k*

*k*
*k*

*k* * ,* *H*

*C* **S**_{i}**.S**** _{j}** (3)

and µ* _{m}*=

*H*

^{m}_{β}=0

This leads to a diagrammatic representation given in^{8}.
The calculation of the coefficients of the γ* _{i}* according
to the diagrammatic method involves two separate
phases.

(a) The finding of all the diagrams or graphs which can be constructed from dashed line connecting the site o and i and straight lines, and the determination of diagrams, in the case of the spinel lattice, whose contribution is non vanishing.

(b) Counting the number of times that a diagram can occur in the spinel lattice. Step (a) has already been accomplished in the S.K work. Step (b), however is very tedious.

In our case, we have to deal with the two Heisenberg
constant couplings: J* _{1}* and J

*between first and second n-n in the spinel system.*

_{2}For each topological form of a given diagram, a full
line can either represent J* _{1}* or J

*. We must, thus derive from each topological form a class of diagrams; each of them represents a term of the series as*

_{2}*)*
*n*
*m*
*and*
*0,1,...,*
*n*
* ,*
*m*
*(*
*J*

*J*1* ^{m}* 2

*= + = for the*

^{n}*order. This is especially the limiting factor in how far one can carry the expansion.*

^{th}In this fashion, we calculated all of the coefficients
required for the calculation of the spin correlation
function γ_{i}*(**i*=1−3*)* in the case of a diluted B-spinel
lattice to order =6, and the results of this calculation
are given in ref.^{25}.

Equation (2) combined with the results in ref.^{25 }allows
the computation of the spin correlation functions γ* _{i}*.

The analytical expressions of γ1* ,*γ_{2}*and*γ* _{3}* are given in
ref.

^{25}.

Since we are interested in estimating critical points,
we have used the P.A methods to study the
dependence of the critical temperature T* _{N}* on the
relative strength of J

*, J*

_{1}*and the ratio of dilution x. T*

_{2}*is estimated as the temperature at which γ*

_{N}_{1}diverges

^{12}. Using [3,4] P.A. we have calculated the ratio

*J*1

*T*_{N}

in
the long range-ordering region of the system
ZnCr_{2}Al2_{-2x}S_{4}. Figure 1 shows the obtained

*J*1

*T**N* (solid
line) against dilution x. In this figure we have
included, for comparison, the experimental results
obtained by neutron diffraction given in^{5}. One can see
the excellent agreement between the theoretical and
experimental results.

0.85 0.90 0.95 1.00

6.4 6.8

x
T_{N} /J_{1}

FIG. 1: Variation of the

*J*1

*T*_{N}

versus the magnetic
concentration x in ZnCr_{2x}Al_{2-2x}S_{4} for 0*.*85≤*x*≤1. The
circles are the experimental points reported in^{5}. The
line is the result obtained from the high-temperature
series expansion extrapolated with the Padé
approximant methods.

The wavelength dependent susceptibility χ*(***q***)* and
correlation function *S**(***q***)* are defined as:

= −
*j*
*,*
*i*

*i*

*B* *e*

*g*
*)*

*(***q** µ β **S**_{i}**.S**_{j}^{q.R}^{ij}

χ ^{2} (4)

and

= −
*j*
*,*
*i*

*e* *i*

*)*
*(*

*S* **q** **S**_{i}**.S**_{j}^{q.R}** ^{ij}** (5)

Where µB is the Bohr magneton, g the gyromagnetic
ratio and **R**** _{ij}** is the separation between the spins i and
j.

In order to obtain a qualitative measure of the
correlation length ξ*(**T**)* for a given temperature T we
144 M. Houssa, M. Hamedoun, N. Benzakour and A. Hourmatallah 2

have expanded the correlation function **S q***(* *)* in a
Taylor expansion about the magnetic reciprocal lattice

**Q** of the given system^{16}.

*]*
*)*
*(*
*)*
*(*
*)[*

*(*
*S*
*)*
*(*

*S* **q** = **Q** 1−ξ^{2} **q**−**Q** ^{2}+0**q**−**Q** ^{4} (6)
Recasting this in the Ornstein-Zernike from, the
following asymptotic form is obtained:

*]*
*)*
*(*
*)*
*T*
*(*
*[*

*)*
*T*
*(*
*)*
*(*
*)* *S*
*(*

*S* _{2} _{2}

2

**Q**
**q**
**q** **Q**

−

= + κ

κ (7)

Where κ*(**T**)*=ξ^{−}^{1}*(**T**)*

In the B-spinel lattice and for the particular case of the
helimagnetic structure with wave vector **Q**=*[*0*0**q]*,
we obtain:

## ( )

^{ù}

êë

é ÷+

ø ç ö è + æ +

= *q* *cos* *q*

*cos*
*)*

*(*

*S* γ* _{aa}* γ

*π γ*

_{ab}*π*

_{ac}1 2 4

**q** (8)

3

1 4

2γ γ

γ*aa* = + is the in-plane correlation, γ*ab*=4γ_{1}+8γ_{2}
is the correlation between neighbor planes and
whereγ*ac*=4γ_{2}+8γ_{3} is the correlation between the
second neighbor planes.

The maximization of *S**(**q**)* with respect to q=q_{0} gives:

*ac*

*q* *ab*

*cos* γ

γ π

4 2

0ö=−

ççèæ (9)

q_{0} is related to the helix angle by:

2
*q*0

θ=π .

Expanding the cosine of equation (8) in the Taylor
expression about q=q* _{0}* and using the equation (6), we
obtain:

ù êê

ë

é− +

÷ = ø ç ö è æ

*ac*
*ab*

*)* *ac*

*q*
*(*
*S*

*a* γ

γ γ ξ

16 8

1 ^{2}

0 2

(10)

where a is the lattice parameter.

The simplest assumption that one can make
concerning the nature of the singularity of the
magnetic susceptibility χ**( q***)* and the correlation
length ξ*(**T**)* is that in the neighborhood of the critical
points the above two functions exhibit an asymptotic
behavior:

## ( )

^{γ}

α

χ*(***q***)* *T** _{N}*−

*T*

^{−}and

^{ξ}

^{2}

*(*

*T*

*)*

^{α}

## (

*T*

*−*

_{N}*T*

## )

^{−}

^{2}

^{ν}(11)

*T*

*represents the critical temperature, deduced by the P.A. methods, γ and ν the critical exponents.*

_{N}Representation of the series expansion of χ**( q***)* and

*)*
*T*

2*(*

ξ by [3,4] P.A. would enable us to find γ^{ and 2}ν
by finding: *LogF**(**y**),**(F(y)* *,* *)*

*dy*
*)**d*
*y*
*y*
*(*

*lim* _{N}^{2}

*y*

*y* *N*

ξ

=χ

→ − with

*N*

*N* *T*

*y* *J*
*T* *and*

*y*=*J*^{1} = ^{1} . We have obtained the values of the

above two critical exponents in the case of the B-
spinel ZnCr_{2x}Al_{2-2x}S_{4}. Using the helix angle θ deduced
from the position of the magnetic satellite of the
neutron diffraction pattern ^{17}, θ(x=1)=71^{0},
θ(x=0.90)=68^{0} and θ(x=0.85)=64^{0}, we have obtained
the central values of γ^{ and }ν for three concentrations
γ=1.382±0.012 and ν=0.691±0.011. These values may
be compared with those of the 3D Heisenberg model,
namely, 1.3866±0.0012 and 0.7054±0.0011^{18-19}. The
agreement is excellent.

On the other hand in figure 2 we show the temperature
dependence of the **S q***(* *)* in the case of ZnCr_{2}S_{4} (x=1).

We observed a strongly developed S.R.O hump
peaking at the wave vector **q****0**^{=}

## [

^{0}

^{0}

^{0}

^{.}^{79}

## ]

. The broad diffuse peak becomes broader and weaker as the temperature is raised, corresponding to the thermal disruption of the magnetic correlation. The accordance with the experimental result obtained by the neutron diffraction is excellent. We note that the S.R.O is fairly well developed at relatively high temperatures,*T≈100K, and may even be present at room*temperature. The thermal variation of set of absolute values of J

*and J*

_{1}*keeping the maximum of*

_{2}

**S q***(*

*)*at the particular wave vector

**q**

**is obtained. This variation is presented in figure 3.**

_{0}0.0 0.4 0.8 1.2

1.05 1.10 1.15 1.20 1.25

q 30K

100K 50K 35K T= 25K

S(q) (u.a)

FIG. 2: Static structure factor **S q***(* *)* of the system
ZnCr_{2}S_{4} for various temperatures along the wave
vector **q**=

## [ ]

^{0}

^{ 0}*. Lines are theoretical results obtained from equation 2 (see text) and the dots are the experimental data obtained in*

^{q}^{5}.

In figure 4 we present the variation of **S q***(* *)* with the
ratio of dilution x in the paramagnetic phase of the
system ZnCr_{2x}Al_{2-2x}S_{4}. This variation is similar to that
with the temperature. The only difference is that the
position of the peak shifts to lower values when x
decreases. This result is in agreement with the
experimental neutron diffraction^{5}. The variation of the

peak position of the S.R.O with the ratio of dilution
and not with the temperature can be linked to the fact
that the lattice parameter in the thiospinel varies with
x according to the Vegard’s rule^{20} but it is independent
of temperature^{21}.

The magnetic correlation length ξ is given by equation 3. In figure 5 the variation of the inverse correlation length

ξ

1 with the temperature

20 40 60 80 100

1.04 1.12 2.24 2.32

(b) (a)

Ji ___

___

T(K)

FIG. 3: Temperature dependence of the absolute
values of exchange integrals in the system ZnCr_{2}S_{4}.
(a) nearest neighbor interactions J* _{1}*. (b) next nearest
neighbor interactions J

*.*

_{2}0.0 0.3 0.6 0.9 1.2

1.04 1.08 1.12 1.16 1.20 1.24

0.60 0.80

q 0.85 0.9 x=1

S(q) (u.a)

FIG. 4: Structure factor **S q***(* *)* for several ratio of
dilution in ZnCr2xAl2-2xS4 in the paramagnetic phase.

The lines are the theoretical results and the dots are
experimental data obtained by neutron diffraction
obtained in ^{5}.

for different x is presented. The variation is linear with the same slope of different composition in the S.G.

region.

20 40 60 80 100 120

1.5 2.0 2.5 3.0 3.5

( *a* / ξ )

T (K) x=0.55

0.60 0.65

0.75

FIG. 5: Temperature dependence of the inverse
correlation length for several values of x situated in
the spin glass region of the system ZnCr_{2x}Al_{2-2x}S_{4}.
An important result exhibited by neutron diffraction
experiments in the thiospinel systems is the non
existence of any anomaly in the correlation length at
the freezing temperature T* _{f}* and the extrapolated values
of ξ

1 at T=0 are finite in the S.G region^{12,13,22}. We
extrapolate the correlation length presented in figure 5
to *T=0. In figure 6 the variation of *ξ(T=0) with x is
presented for two sets of parameters, (i) n-n
interactions only and (ii) n-n and n-n-n interactions.

We know, on physical grounds, that if the magnetic
concentration fell below the percolation concentration
(for a given lattice), the macroscopic connectivity of
the magnetic lattice would break down such that the
spin correlation length would reduce to zero. This
critical behavior is deduced from figure 5. The
percolation threshold is considered as the
concentration at which ξ=0. It is equivalent to the
concentration at which there is no magnetic
connection between spins. The obtained values are
x_{p}=0.27 when only J* _{1}* is considered and 0.23 when
both

*J*

*and J*

_{1}*are considered. These values are in agreement with those obtained by the Monte Carlo method*

_{2}^{14}and the magnetic measurements

^{15}.

146 M. Houssa, M. Hamedoun, N. Benzakour and A. Hourmatallah 2

0.15 0.30 0.45 0.60 0.75 0.0

0.2 0.4 0.6 0.8

(b) (a)

/a)(=ξ

x

FIG. 6: Variation of the correlation length with x in
ZnCr_{2x}Al_{2-2x}S_{4} at T=0. (a) Only J_{1} is considered. (b):

Both J* _{1}* and J

*are considered.*

_{2}**III. CONCLUSIONS:**

The first three spin correlation functions for the
diluted B-spinel lattice ZnCr_{2x}Al_{2-2x}S_{4 } where
determined with the nearest and next- nearest neighbor
interactions to order 6 in β by the high-temperature
series expansion.

High-temperature series expansion extrapolated with
Padé approximants is shown to be a convenient
method to provide valid estimations of critical
temperatures for magnetic system^{23}. By applying this
method to the γ_{1}, we have estimated the long-range
order region of ZnCr_{2x}Al_{2-2x}S_{4}. The obtained results
are in good agreement with those obtained by
experimental neutron diffraction. The critical
exponents of the magnetic susceptibility γ^{ and the}
correlation length ν are found equals to 1.382±0.012
and 0.691±0.011 in the whole range of concentration

1 85

0*.* ≤*x*≤ . These values are compatible with those of
3D Heisenberg model. According to Harris criterion^{24},
since ZnCr_{2}S_{4} is a good 3D Heisenberg system, the
critical exponent α of the specific heat is less than
zero^{18}, hence, the critical exponents are unaffected by
dilution.

On the other hand the variation of **S q***(* *)* and ξ with
temperature and magnetic site dilution x is derived.

We find that for a given ratio of dilution the thermal
variation of the magnetic structure remains peaked at
the wave-vector corresponding to the magnetic
structure. The set of the nearest-neighbor and next-
nearest neighbor interactions, J* _{1}* and J

*respectively, respecting this behavior are deduced. For the pure system (x=1), the absolute values of J*

_{2}*and J*

_{1}*exhibit an exponential decay with the temperature. The position of the peak in*

_{2}

**S q***(*

*)*shifts to lower

**q**with increasing dilution. These features are in agreement

with neutron diffraction experiments on the system
ZnCr_{2x}Al_{2-2x}S_{4}.

The obtained inverse correlation length ξ

1 decreases
linearly with the temperature and the extrapolated
values at T=0 are finite for the concentration in the
spin glass region *x*≤0.80. The variation of the
correlation length with x at T=0 gives us a method for
the estimation of the threshold percolation x_{p}. The x_{p}
is considered as the concentration at which ξ
vanishes. The obtained values are x_{p}=0.27 when only
*J** _{1}* is considered and 0.23 when both J

*and J*

_{1}*are considered. These values are comparable with those obtained by the Monte Carlo method and the experimental phase diagram in the T-x plane of ZnCr*

_{2}_{2x}Al

_{2-2x}S

_{4}obtained by the a.c and d.c susceptibility.

1 H. E. Stanley, in Disordered Systems and Localization, Vol. 149 of Lectures Notes in Physics, edited by C. Castellani, C. di Castro and L. Peliti (Springer, Berlin 1981).

2 K. Binder and P. Young, Rev. Mod. Phys. 58 (1986) 137.

3 H. Malleta, G. Aeppli and S. M. Sapiro, Phys. Lett.

48 (1982) 1490.

4 J. R. de Sousa and Douglas F. de Albuquerque, Phys.

Rev. B48. 16 (1993) 484.

5 M. Hamedoun, A. Wiedenmann, J. L. Dormann, M.

Nogues and J. Rossat-Mignod, J. Phys. Solid State Phys. 19 (1986) 1783.

6 D. Staufer, Introduction to Percolation Theory (Taylor and Francis, London, 1985).

7 H. E. Stanley and T. A. Kaplan, Phys. Rev. 16, (1966) 981.

8 H. E. Stanley and T. A. Kaplan, Phys. Rev. 158, (1967) 537.

9 G. S. Rushbrook and P. J. Wood, J.Phys. Mol. 1 (1958) 257.

10 R. V. P. Singh and R. L. Glenister, Phys. Rev. B 46 (1992) 11871.

11 A. Wiedenmann, P. Burlet, H. Scheur and P.

Convert, Sol. State, Commun. 38 (1981) 129.

12 A. Wiedenmann, M. Hamedoun and J. Rossat.

Mignod, J. Phys.: Solid. State Phys. 18 (1985) 2549.

13 D. Fiorani, S. Viticoli, J. L. Dormann, J. L.

Tholence and A. P. Murani, Phys. Rev. B 30 (1984) 2776.

14 D. Fiorani, L. Gastaldi, A. Lapiccirela, S. Viticoli and N. Tomassimi, Sol. Stat. Commun. 32 (1979) 831.

15 M. Alba, J. Hammann and M. Nogues, J. Phys. C:

Solid State. Phys. 15 (1982) 5441.

16 K. Kawasaki and R. A. Thahir-Kheli, Phys. Rev. B.

15 (1977) 2741.

17 M. Hamedoun, A. Rachadi, A. Hourmatallah, D. El Allam and A. Benyoussef, J. Status Solidi (b), 191 (1995) 503.

18 For a review, see Collins, M. F 1989, Magnetic.

Critical. Scattering (Oxford: Oxford University Press).

19 J. C. Le Guillou and Zinn-Justin, J. Phys. Rev. Lett.

2 (1977) 95.

20 E. Agostinelli, C. Batistoni, G. Mohogno and M.

Nogues, J. Phys. Chem. Solids. 50 (1989) 269.

21 M. Hamedoun, A. Hourmatallah, S. Sayouri and A.

Chatwiti, J. Phys: Codens. Matter, 7 (1995) 5359.

22 D. Fiorani, S. Viticoli, J. L. Dormann, J. L.

Tholence, J. Hammann, A. P. Murani and J. L.

Soubcyroux, J. Phys. C: Solid state. Phys. 16 (1983) 3175.

23 M. C. Moron, J. Phys. Condens. Matter, 8 (1996) 11141.

24 A. B. Harris, J. Phys.C: Solid State Phys. 7 (1974) 1671.

25 M. Hamedoun, M. Houssa, N. Benzakour and A.

Hourmatallah, Physica B 270 (1999) 384.